Macromolecules 1995,28, 4173-4178
Mechanism of Cis-Trans Thermal Isomerization of Polyacetylene Yoshikazu Tanabe* and Hiroko Kyotani National Institute of Materials and Chemical Research, Tsukuba 305, Japan
Kazuo Akagi and Hideki Shirakawa Institute of Materials Science, University of Tsukuba, Tsukuba 305, J a p a n Received January 24, 1995; Revised Manuscript Received March 22, [email protected]
ABSTRACT: Isothermal cis-trans isomerization of polyacetylene (PA) films proceeds according to a stretched-exponential function of time with a n exponent a (0 < a < 1). A mechanism is proposed for the cis-trans isomerization. Cis-trans isomerization of PA occurs under the condition t h a t the molecular axis is almost fixed. The interspace-diffusion model is effective in simply describing the intermolecular cooperative motions of neighboring chains t o avoid the intermolecular constraints for cis-trans isomerization motion. If a n interspace appears in the neighborhood of a cis bond (or moving unit of cis state), this cis unit is assumed to change to the trans state instantaneously. Using the continuous-time random walk model; the decay of survival probability of a cis unit can be expressed by the stretchedexponential function under the assumption of the distribution of activation energy for cis-trans isomerization. The relationship between the two-state model and the interspace-diffusion model is discussed.
1. Introduction Structure and properties of a polyacetylene (PA) film are strongly affected by the aging temperature of the catalyst. High dc conductivity and stability1s2 were found in a PA film synthesized with an aged catalyst at high temperature (for example, over 373 K). Mechanical properties such as Young’s modulus, tensile strength, and stretchability were also improved3 compared to the previous Shirakawa PA film The difference in the conduction mechanism between highly stretchable PA (hs-PA) and S-PA was discussed based on the frequency (w)and temperature (T> dependence of the complex conductivity ~ * ( o Reducing ).~ o*(w) and o by using the dc conductivity a(O), a master curve was obtained for hs-PA but not for S-PA. The difference in the conduction mechanism between hs-PA and S-PA arises from their morphological dissimilarities. Isothermal cis-trans isomerization of PA has been studied by infrared spectroscopy (IR).6,7Differential scanning calorimetry (DSC) also gives various information on the isomerization. A two-state model, in which population probabilities for cis and trans states are assumed to change through the forward and backward reactions, was used to analyze DSC curves.8 The enthalpy difference between the two states and the activation energy were determined from this analysis. Kyotani et al. also studied the isothermal cis-trans isomerization behavior by means of DSC.g By defining the isomerization ratio y by y = ( A H 0 - AHJAHo where A H 0 and AHt are the heats of isomerization for the aspolymerized film and for the film which was preheated for t hours, respectively, the experimental data were represented by the following stretched (fractional)exponential function,
where ko and a are constant, and 0 < a < 1 experimentally. The temperature dependence of ko gives an
* To whom correspondence should be addressed.
published in Advance ACS Abstracts, May 1, 1995. 0024-9297/95/2228-4173$09.00/0
activation energy of ca. 30 kcavmol. Recently it was found that the previously reported IR data can also be described by eq 1.l0 This replotting gave an activation energy of ca. 28 kcavmol independent of cis content. Equation 1 with 0 < a < 1 is the same function as the Kohlrausch-Williams-Watts (Kww) function in the field of dielectric relaxation. If a > 1, eq 1 is the same as the Avrami equation in the field of polymer crystallization from the molten state. In the case of isothermal cis-trans isomerization in PA, a is determined experimentally to be less than unity. The above-mentioned two-state model suggests a single (simple)-exponential decay for the isothermal isomerization,8 which is different from eq 1. On the other hand, nearly the same activation energy was derived by the two methods (heating rate dependence of peak temperature for cis-trans isomerization and the temperature dependence of ko in isothermal experiments). This paper is concerned with the mechanism of cistrans isomerization of PA and also with the derivation of eq 1 from this mechanism. The relationship with the two-state model is also discussed. 2. Interspace-DiffusionModel
X-ray diffraction studies have shown a continuous and monotonous shift of the initial diffraction of cis crystallites.11J2 There is no direct evidence for the coexistence of cis and trans crystallites. The overall crystal structure is maintained during the partial isomerization within a chain. In other words, the partial isomerization of a chain does not change the crystallite lattice pattern. The phenomenon that chains with different chemical structures are drawn into another crystal structure is called isomorphism in crystals and is seen in copolymers and so on. For the molecular motion related to the thermal isomerization, Yamabe et al.13 proposed a crankshaft motion of the -(CH=CH)- unit around two carbon-
0 1995 American Chemical Society
Macromolecules, Vol. 28, No. 12, 1995
4174 Tanabe et al.
Figure 1. Model of intramolecular correlated vibrational/ rotational motions for cis-trans thermal isomerizationof PA.
carbon double bonds in cis-transoid form which is the most preferable conformation in as-polymerized PA films. They found that the energy barrier for the rotation to change the dihedral angle of one cis-transoid monomer unit by 180" is ca. 1 eV (23 kcallmolj. The calculation, however, did not include the effect of steric constraints imposed by the crystal lattice for this cistrans isomerization in the solid state. As suggested by X-ray results, the molecular axes do not move very much during thermal isomerization. This means that the effect of steric constraints during isomerization is very large and the intramolecular motions are limited within small spaces around the molecular axis. The intramolecular motions for cistrans isomerization in the solid state would consist of vibrationslrotations of bonds or bond sequences around the molecular axis. An example is described in Figure 1. The part of the chain above the double bond A and the part of the chain below the double bond B are considered to be hard bodies (denoted by dashed lines). These parts vibratehotate cooperatively around bond A and bond B with the condition of inverse direction. Simultaneously the reorientation andor torsions of the molecular axis occurs; otherwise, the molecular axis declines. This type of cooperative internal rotation is possible between bonds A and C and other pairs of bonds. Of course, other kinds of bond motions would be possible for intramolecular correlated vibrationall rotational motions around the molecular axis. Even if the intramolecular cooperative motions such as shown in Figure 1exist, the cis-trans isomerization
Figure 2. Model of intermolecular cooperative vibration' rotation of neighboring chains. The formation of interspaces is essential.
does not occur because of the steric hindrances among chains in the solid state. Intermolecular correlated motions of neighboring chains are needed for thermal cis-trans isomerization. There are many possibilities for cooperative intermolecular motions responsible for cis-trans isomerization. Among them, the common essential point is to make space between chains, which make the cis-trans thermal isomerization possible. Figure 2 shows an example in which the incoherent intermolecular motions of chains make a space between neighboring chains. If these spaces are made by thermal fluctuations, a part of the neighboring chain is transformed from cis to trans states. Hereafter these spaces are called interspaces. Suppose that the PA film contains mobile interspaces, which can move through thermal motions of PA chains. If an interspace reaches the site of a cis bond (or an elementary moving unit for cis-trans isomerization, if it exists), this cis bond changes to the trans state instantaneously. The diffusion of interspaces is essential in this model and is not necessarily limited to one dimension (along chain axis). Interspaces can diffuse in the directions parallel and perpendicular t o the PA chain. The similar model was discussed by Shlesinger and Montroll14to derive the KWW polarization decay function similar to eq 1. Let a cis bond (or moving unit) be situated at the origin of a postulated lattice of V sites. Consider that N independent mobile interspaces are also on this lattice, but not initially at the origin. The cis content P,(tj at time t is the survival probability of cis units not yet transformed by meeting with an interspace. Let F(x,t)be the probability density at time t that an interspace originally at x reaches the origin for the first time. The probability that the interspace does not reach the origin in the time interval (0,t) is then given by [ 1- Jt$(x,t) dt]. The survival probability
Cis-Trans Thermal Isomerization of Polyacetylene 4176
Macromolecules, Vol. 28, No. 12, 1995
P,(t) of cis units is expressed as V
C - C n [ l - htF(X,,t)dtl
where y(z,p)is the first kind of incomplete r function.ls The barrier density (eq 8) approaches a delta-function In this case q(t) if the halfwidth TO 0, i.e., a approaches a Markoffian process (eq A19). When vt is large, eq 12 gives
Q=l i = l
where U ( X I , X P , ...,XN) is the initial distribution function of interspace positions. If the interspaces are initially randomly distributed, U ( X 1 , X 2 , ...,XN) = lNN,then The Laplace transform of eq 13 is approximated by
q * ( u ) E 1- (-' r + 1L- (agv ) ( a # 1) sinmv
under the condition that u is small, where the Laplace transform of q(t)is given by
in the thermodynamic limit that N and V becomes infinite with fixed c, where c = N N is the concentration of interspaces. It is convenient to use the continuous-time random walk (CTRW) model by Montroll and Weiss15 in order to calculate the first-passage-time probability density F(x,t). The CTRW is composed of an alternation of steps and pauses. The detailed derivation is briefly shown in the Appendix. In CTRW, the pausing-time (or hopping time) distribution function q(t)plays an essential role. In the case of interspace diffusion, q(t)is assumed to be based on a distribution of activation energy barriers. For a distribution of barrier heights,
E, where EOand kgTo are the peak position and the width of the distribution ofg(E), respectively. Equations 6-8 yield
When a > 1, eq 14 is approximated as q * ( u ) E 1 [&(a - l)l(u/v) and P,(t) is expressed by a singleexponential function. When a = 1, q*(u) = 1 - (u/v) ln(1 + d u ) and it is impossible to get K(t) and P,(t) analytically.
3. Discussion DSC curves were analyzed by us based on the twostate model.8 A relationship exists between the twostate model and the interspace-diffusion model, which is discussed below. The information derived by the interspace-diffusion model is also discussed. Time-Dependent Rate Constant. From eq 3, dPc(t)/dt = -cK(t) P,(t)
The rate constant K(t)depends on time t , which means this system has a memory effect. Therefore, eq 20 can be replaced by
dP,(t)ldt = -cLt4(t--t) P,(t) dr
Substituting eq 9 into eq 5,
q(t)= (dv")t-l-"y(af 1,vt)
where +(t)is the memory function. This function is
4176 Tanabe et al.
Macromolecules, Vol. 28, No. 12, 1995
related to K(t) as in eqs 22 and 23.
TEMPERATURE ( K )
If this 4(t) is described by a delta-function, no memory effect exists. Sequential transitions described by CTRW will make the transition rate of the primary relaxation process time-dependent (different from a delta-function). In the interspace-diffusion model, the distribution of the activation energy causes a non-Markovian nature of the pausing-time distribution function as shown in eq 5. Relationship between the Two-StateModel and the Interspace-DiffusionModel. The two-state model previously analyzed8 is represented by
To = 300 K
b = 30 (kcallrnol) q = 10 ('Urnin)
Figure 3. Effect of TOon DSC curve. TOmust be selected below 100 K. Calculated using eqs 25 and 26 with V I = 1014 W1),Eo = 30 (kcaYmol),q = 10 (Wmin), and a = 0.5. TEMPERATURE ( K )
where kf = W exp(-EdkBr), P, Pt = 1, and W is the preexponential factor (attempt frequency). Eo and E are the barrier height and energy difference between cis and trans states, respectively. From a comparison of eqs 20 and 24, it is clear that the interspace-diffusion model is characterized as (1)E being very large and exp(-E/ kBT) infinitely small and then the second term in the right-hand side of eq 24 is neglected and (2) the forward rate constant kf being time-dependent. In the two-state model, the distribution of the activation energy is not taken into account, while in the interspace-diffusion model, the backward reaction from trans to cis states is neglected. DSC Curve Based on the Interspace-Diffusion Model. DSC is measured under the condition of constant heating rate q = dTIdt. By changing time variable t to temperature variable T,eq 20 gives
u, =1014(s-"1 Eo = 30 (kcallrnol) q = 10 ('Clrnin) To=lO(K) 0c.l
Figure 4. Effect of the exponent a on the DSC curve. Calculated using eqs 25 and 26 with V I = 1014(s-I), Eo = 30 (kcaUmol), q = 10 ("C/min), and TO= 10 (K).
At the peak position T = Tp in the DSC curve, the following relation is derived from eq 20 after changing t to T. (v/q)" =
+- a - 1
[a? d o
The right-hand side of eq 28 is nearly constant with changing q. From (vlq)u= const.,
where T = TO qt and v1
The observed DSC curve is proportional to dPddT. In numerical calculation, care must be taken of To. Figure 3 shows the TOdependence of the DSC curve. The effect from TOappears largely at TOabove 100 K. The parameter a has a large effect on the peak position and the width of the DSC curve for cis-trans isomerization, as shown in Figure 4. As a decreases from 1 to 0.5, the peak position shifts to a higher temperature (from 410 to 440 K) and the width becomes broader. The case of a = 1 apparently corresponds to the two-state model with E =.
+ EdkBTpx const.
Equation 30 indicates that the q dependence of peak position Tpgives the activation energy Eo. This method does not depend on the values of a. This is the reason why the two-state model and the interspace-diffusion model give nearly the same activation energy (ca. 30 kcallmol for cis-trans isomerization of PA). The activation energy does not depend on the polymerization condition^.^ The activation energy reflects the energy barrier for the rotation to change the dihedral angle of one cistransoid monomer unit by MOO, because interspace diffusion is activated by the main-chain motions. Its energy barrier calculated by Yamabe et al.13 is ca. 23 kcallmol which is not contradictory to our result. Exponent a. The temperature dependence of the exponent a is shown in Figure 5, which has been measured by DSCg and IR6 methods. The value of a slightly increases with temperature, as suggested by eq 11. As a is nearly 0.5, TOis about 800 K. The width of the activation energy distribution is characterized by
Cis-Trans Thermal Isomerization of Polyacetylene 4177
Macromolecules, Vol. 28, No. 12, 1995
model and the interspace-difision model was discussed. The interspace-diffusion model takes into account the correlation of cis unit motions (the distribution of the activation energy). The experimental temperature dependence of the exponent a is not inconsistent with the interspace-diffusion model.
1 0 , A :
400 TEMPERATURE ( K )
Figure 5. Temperature dependence of a for various PA films, measured by DSCS and IR6methods.
k ~ T o= 1.6 kcal/mol which is a rather small fluctuation compared to Eo x 30 kcal/mol. Effect of c. The effect of c on t-l is very interesting changes an order of (see eq 19). If a is 0.5, magnitude when c changes by more than 3 times. The exothermic peak position of cis-trans thermal isomerization shifts to 20-30 K lower temperature, as suggested in Figure 6 of ref 8, because the preexponential factor W in ref 8 is related to the inverse of z and to elia. Although the calculation in ref 8 corresponds t o the case of a = 1 (see Figure 4), the qualitative nature is nearly the same. Experimentally, S-PA shows a higher temperature peak position around 443 K in cis-trans thermal isomerization. On the other hand, hs-PA has a lower temperature peak position around 413 K. As suggested in ref 22, hs-PA has a more disordered structure of crystallites than that of S-PA. A more disordered structure of crystallites gives a larger value of c and a lower temperature of the exothermic peak. This seems to be one of the reasons why hs-PA shows a lower temperature peak position than that of S-PA since there is no large difference between a’s of S-PA and hs-PA. S-PA has the two DSC exotherms near 440 K (main peak) and 420 K (shoulder). These have nearly the same activation energy. Accordingly, the difference of these two peak positions can be attributed to the difference in c . That is, S-PA has two kinds of solid structure (the more and less ordered structures). The same result has been derived in ref 22.
Appendix. Continuous-Time Random Walk CTRW was introduced by Montroll and Weiss15 to consider the situation that the jumps of random walker do not occur at regular time intervals but are made with the pausing-time distribution (or hopping time distribution). Random walk at regular time intervals on a periodic lattice is described by the probability P,(s) of being at site s after n steps.
P,+,(s) = >(s-s’)
where p ( s ) is the probability of a single jump having a displacement s and C&) = 1. Let F,(s) be the probability that a random walker reaches site s for the first time at the nth step. n
+ C F j j ( S ) Pn-j(O)
By introducing the generating functions, m
eq A1 gives
For a finite lattice with periodic boundary conditions,
In order to explain the stretched-exponential function with exponent a (0 < a < 1)which has been found in the isothermal cis-trans isomerization behavior of PA films, the interspace-diffusion model was discussed. As X-ray diffraction experiments suggested, the cis-trans thermal isomerization of PA occurs under the condition of the molecular axis being nearly fixed. Not only intramolecular cooperative motions of cis bonds (or units) but also intermolecular cooperative motions among neighboring chains are unavoidable. The interspace-diffusion model is proposed to simply describe the intermolecular cooperative motions of neighboring chains. If an interspace reaches a cis bond (or moving unit of cis state), this cis bond changes to trans bond instantaneously. Using a continuous-time random walk model, the decay of survival probability of cis units can be expressed by the stretched-exponential function under the assumption of the distribution of the activation energy for cis-trans isomerization. The relationship between the previously analyzed two-state
and k = 2xrlN (r = integer). The probability density qn(t)for the occurrence of the nth step (jump) at time t is
where ~ ( is t )the pausing-time distribution function (the hopping time distribution function). The probability density F(s,t)for reaching site s for the first time at time t is m
F(s,t) = p
y s ) +,(t)
The probability density R(s,t)for reaching site s (or to just arrive at s ) a t time t (not necessarily for the first
Macromolecules, Vol. 28, No. 12, 1995
4178 Tanabe et al.
A1 = vp exp(-E,IkBT)
time) is (All) The probability P(s,t)of being at s at time t is
P(s,t)= S,'R(s,t)Y(t-t) dz
Y ( t )= 1 - htq(t) dt (A131
where Y represents the probability that a walker remains fixed in time interval (0,t). The probability P(s,t)includes the effect of staying at s during t - t after just reaching at s. The Laplace transform of P(s,t) is given by
F*(s,u)= H[s,q*(u)l (A151 Using eqs A8 and A15, the Laplace transform of K(t) becomes
Here, (A171 was used since C,p(s-s') = 1 in eq A5. For a three-dimensional simple cubic lattice,l5
when z approaches unity. The pausing-time distribution function q(t)introduces a memory function into the master equation (ME) of P(s,t),16which is called the generalized master equation (GME). When +(t) is described by a Poisson distribution function,16
~ ( t=)1, exp(-A,t) with
where E1 is an activation barrier height, vp the prefactor attempt frequency, k B the Boltzmann constant, and T the absolute temperature. No memory effect appears in this case. Generalization of Montroll-Weiss CTRW was made by Scher and Laxlg using q ( s , t )depending on hopping distance. This GCTRW is proved to be the same with GME by Klafter and Silbey.20,21
References and Notes
= J/-v(z) dt
G(Oq)= 1.516 - (3/~)(3/2)'"(1 - z)'"
(1) Naarmann, H.; Theophilou, N. Synth. Met. 1987,22,1. (2) Tsukamoto, J.; Takanashi, A.; Kawasaki, K. Jpn. J . Appl. Phys. 1990,29,125. (3) Akagi, K.; Suezaki, M.; Shirakawa, H.; Kyotani, H.; Shimomura, M.; Tanabe, Y. Synth. Met. 1989,28,D1. (4) Ito,T.; Shirakawa, H.; Ikeda, S. J . Polym. Sci., Polym. Chem. 1974,12,12. ( 5 ) Ito, K.; Tanabe, Y.; Akagi, K.; Shirakawa, H. Phys. Reu. B 1992,45. . . 1246. (6) Ito, T.; Shirakawa, H.; Ikeda, S. J . Polym. Sci., Polym. Chem. 1975.13,1943. (7) Chen, Z.-G.; Shen, Z.-Q.; Lin, M.; Shi, M.-X.; Hummel, D. 0. Mukromol. Chem. 1987,188,2697. (8) Tanabe. Y.:Kvotani. H.: Shimomura, M.: Akaei, K.: Suezaki, M.; Kasai, T.; Shirakawa, H. J . Poiym: Sci.;Polym. Phys: 1991,B29,501. (9) Kyotani, H.; Shimomura, M.; Ito, K.; Tanabe, Y.; Zhang, Y.X.; Akagi, K.; Shirakawa, H. Rep. Prog. Polym. Phys. Jpn. 1991,34,141. Kyotani, H.; Shimomura, M.; Ito, K.; Tanabe, Y.; Zhang, Y.-X.; Akagi, K.; Shirakawa, H. J . Polym. Sci., Polym. Phys. 1995,B33,581. (10)Tanabe, Y.; Kyotani, H.; Akagi, K.; Shirakawa, H. Rep. Prog. Polym. Phys. Jpn. 1994,37,325. (11) Robin, P.; Pouget, J. P.; Comes, R.; Gibson, H. W.; Epstein, A. J. Phys. Rev. B 1983,27,3938. (12) Perego, G.;Lugli, G.; Predretti, U.; Cesari, M. Makromol. Chem. 1988,189,2671. (13) Yamabe, T.; Akagi, K.; Ohzeki, K.; Fukui, K. J . Phys. Chem. Solids 1982,43,577. (14) Shlesinger, M. F.; Montroll, E. W. Proc. Nutl. Acad. Sci. U S A . 1984,81,1280. (15) Montroll, E. W.; Weiss, G. H. J . Math. Phys. 1965,6 , 167. (16) Kenkre, V. M.; Montroll, E. W.; Shlesinger, M. F. J . Stat. Phys. 1973,9 , 45. (17) Pfister, G.; Scher, H. Adu. Phys. 1978,27,747. (18) Bendler, J. T.; Shlesinger, M. F. Macromolecules 1985,18, 591. (19) Scher, H.; Lax, M. Phys. Rev. B 1973,7, 4491. (20) Klafter, J.; Silbey, R. Phys. Rev. Lett. 1980,44,55. (21) Klafter, J.;Silbey, R. J . Chem. Phys. 1980,72,843. (22) Kyotani, H.;Shimomura, M.; Tanabe, Y.; Akagi, K.; Kasai, T.; Zhang, Y.-X.; Shirakawa, H. J . Polymer Sci., Polymer Phys. 1996,B33,587. I